Important emission lines of some lanthanide ions.
Rare earth‐doped glasses find applications in numerous photonic devices including color displays, infrared solid‐state lasers, and indicators, among many. In this chapter, we will present and discuss several luminescent glasses doped with rare earth ions in their trivalent form (RE3+) with general background and technological perspectives. Initially, we begin with a short introduction of RE3+ electronic energy‐level structure in solids followed by the discussion of structural feature of glass lasers. While the lasing properties are mainly governed by the solubility of the ions and phonon interactions, the issue of ion interactions in solid hosts will be addressed since they hardly depend on the type of materials. Spectroscopic properties of Nd3+‐doped phosphate glasses are discussed in the framework of Judd‐Ofelt theory. Rare earth‐doped optical amplifiers are tackled from a technological point of view, as well as luminescent solar concentrators for enhancement of solar efficiency.
- rare earth ions
- optical amplifiers
- solar concentrators
A large number of ions from the lanthanide (rare earth) and actinide groups of periodic table exhibit laser action when doped into a large number of host crystals or glasses. The construction of high‐power crystalline lasers requires substantial crystal sizes. In practice, crystals are grown by the small seed crystals while pulling the larger crystal from the melt. These methods are very difficult if larger crystals are needed. When glasses are used as host media, the environments of the ions vary much more than in a crystalline material because of the random structural character of the glass matrix. All glass lasers until present date have used trivalent lanthanides as the active ions. Glass plays many varied roles in rare earth laser systems, as it can be made with uniformly distributed rare earth concentrations and has great potential as a laser host medium. In addition, rare earth‐doped fibers have received growing attention recently. They can be used as amplifiers in optical communication systems and as optical sources. Glass lasers are substantially inhomogeneously broadened, and usually present more broader line width than Nd:YAG ones. The laser transition line width and shape typically vary from one glass to another glass matrix. In this way, innovation of glass lasers remains a vibrant area in the development of science and technology. The luminescent glass materials are used to develop solid‐state lasers operating in visible and NIR regions due to their potential applications in the fields of medical, eye safe lasers, atmosphere pollution monitoring, energy converters and telecommunications. Sharp fluorescent lines, strong absorption bands, and reasonable high quantum efficiency will determine the adequacy of laser material.
In this contribution, the introduction consists of brief review of electronic energy‐level structure of RE3+ in solids, structural features, and general considerations in laser glasses. Laser glasses and amplifiers are studied to know the spectroscopic parameters using spectroscopic techniques. Especially, the current achievements on Nd3+‐doped phosphate glass lasers will be discussed and numerous data will be presented. Er3+‐doped glass fiber amplifiers subject will also be addressed. Finally, we will discuss rare earth‐based luminescence concentrators for photovoltaic applications.
1.1. Rare earth ions as luminescent centers
Trivalent rare earth ions are well known for their special optical properties, which result from the fact that the electronic transitions within the 4f shell occur at optical frequencies. The 4f shell is shielded by the completely filled 5s and 5p shells, so the frequencies of the transitions are almost independent of the host. Generally, the electric dipole transitions are forbidden due to equal parity of the electronic levels within the 4f shell. Those transitions are possible in solids that have slightly mixed odd‐parity wave functions. As a result, the absorption and emission cross sections are small (~10-20 or 10-21 cm2), and the lifetime of the luminescent level is relatively long ranging from microseconds to several milliseconds. The influence of the electric field around the ions removes the degeneracy of the 4f levels, resulting in a Stark splitting of the levels. Figure 1 shows the energy levels of the trivalent lanthanide ions (4f configurations). This figure provides useful information to predict and/or to make a proper assignment of the emission spectra corresponding to trivalent rare earth ions in crystals or glasses.
The energy levels of the 4f shell arise from spin‐spin and spin‐orbit interactions and are often denoted using Russell‐Saunders notation 2S+1LJ [1, 2], in which S is the total spin angular momentum, L is the total orbital angular momentum, and J is the total angular momentum. There exist 14 rare earth elements all having a different number of electrons in the incompletely filled 4f shell. However, due to the shielding by the outer lying shells, the magnitude of the splitting is small, resulting in relatively narrow lines.
Table 1 displays some important emission transitions of rare earth ions and their technological interest. More general views about the spectra and energy levels of rare earth ions can be found in literature [9–12]. The large number of excited states that are suitable for optical pumping and subsequent decay to metastable states having high quantum efficiencies and narrow emission lines is favorable for achieving laser action.
|RE3+ ions||Transitions||Wavelength (nm)||Application|
|Pr3+||1G4→3H5||1300||Optical amplifier |
|Nd3+||4F3/2→4I11/2||1064||Solid‐state lasers |
|Eu3+||5D0→7F2||615||Displays, lighting |
|Dy3+||6F11/2+6H9/2→6H15/2||1300||Optical amplifier |
|Er3+||4I13/2→4I15/2||1530||Optical amplifier |
|Tm3+||3H4→3F4||1480||Optical amplifier |
1.2. Glasses for lasers and amplifiers: structural features
Glasses are widely used nowadays and present several applications in different fields of life. There are several definitions for glassy materials. Grouping them one can define glass as an inorganic product of melting which has been cooled to a solid without crystallization . It means that glass looks like an undercooled liquid. An undercooled liquid can crystallize at any moment but at room temperature it is not possible. Therefore, glass is an amorphous material as it does not exhibit long range order of atoms in a lattice. The transition of a glass melt to a crystallized state at the crystallization temperature does not take place if the cooling of the glass is fast. Below the crystallization temperature, glass behaves like a fluid down to the transformation temperature. Below this temperature, glass has the properties of a solid. Glass can also be defined as an amorphous solid lacking completely, in long range, periodic atomic structure and exhibiting a region of glass transformation behavior.
In general, glasses can be prepared either from high quality, chemically pure components or from a mixture of far less pure minerals. The batch materials can be divided in to five categories depending on the property of components used in the glass preparation: (1)
These oxide glass formers play an important structural role in glasses when used as network or intermediate oxide modifiers. Thus, the oxide network modifiers will create strong bridging oxygen (BO) bonds in between the glass‐forming polyhedra and weak nonbridging oxygen (NBO) bonds (see in Figure 2a). Moreover, the oxide modifiers will control many useful properties, lowering the melting temperature that is highly useful for developing technologically used glasses. The intermediate oxides also modify glass properties due to their coordination numbers and bond strengths in between the network formers and network modifiers. Table 2 reports some of the oxide‐based modifier glasses for realization of structure influence on various properties.
|Glass composition||D (g/cm3)||Tg (°C)||nd||τ (ms)|
Owing to superior physical properties such as high thermal expansion coefficients, low melting and softening temperatures, and high ultraviolet transmission, phosphate glasses have several important attributes over conventional silicate and borate glasses. However, the poor chemical durability of these early optical glasses has temporarily discouraged for their further development. Interest in the amorphous alkali phosphates was stimulated in the 1950s by their use in a variety of industrial applications, including sequestering agents for hard water treatments and dispersants for clay processing and pigment manufacturing . Studying such materials, Van Wazer  established the foundations for much of our current understanding of the nature of phosphate glasses. Kordes and co‐workers [21, 22] re‐examined the alkaline earth phosphate glasses, including UV‐transmitting compositions and observed some “anomalous” trends in properties.
Phosphate glasses have unique characteristics that include high transparency, high thermal stability, low refractive index and dispersion, and high gain density due to high solubility for lanthanide ions and hence find growing field of applications [23–26]. An important step in laser glasses occurred in 1967 when phosphate‐based compositions were first explored . Several phosphate glasses find considerable applications in optical data transmission, detection, and sensing . The phosphate glasses also find applications in fast ion conductors, optical filters, reference electrodes, stable storage medium for immobilizing high‐level nuclear waste  and as additives in the manufacturing of insulating polymeric cables. Certain phosphate vitreous electrolytes are being used increasingly in electrochemical sensors, in prototype batteries, and in electrochemical devices. There have been many excellent reviews of structural studies on phosphate glasses including that of Van Wazer [20, 30, 31]. A schematic structure of different atomic neighborhoods (covalent and ionocovalent) in rare earth (Er3+)‐doped phosphate glass is shown Figure 2b.
The large concentration of lasing atoms can be doped easily into different glasses, which can be made in different shapes and sizes depending on technological needs. The high‐power laser threshold is possible from the ions‐doped glasses compared to the same ions‐doped crystal due to their large absorbing capability of incident energy and energy level broadening. The electronic transitions of rare earth ions have 4f‐4f and 4f‐5d configurations, which are weakly affected by the host material, since the 4f electrons are effectively screened by outer, filled electron shells. Thus, these transitions cause absorption and fluorescence patterns from the ultraviolet (UV) to infrared regions and they are narrow. Two important aspects of the optical behavior of rare earth ions are determined by the host material. One is the electric dipole transitions which occur between 4f states are strictly forbidden for an isolated ion, since the parity of the electronic configuration must change with an electric dipole transition. However, the strengths of these electric dipole transitions remains relatively weak due the perturbative nature of the admixing states, and as consequence, the radiative lifetimes of excited rare earth ions can be relatively long (∼10-3 ms). Another aspect is related to the nonradiative rates originated from relaxation of the excited states of the rare earth ions, which is determined by the host material. Recently, Babu et al.  had studied different fluorophosphate glasses doped with 0.5 mol% of Er3+ ions through the Judd‐Ofelt and McCumbers theories for potential broadband optical fiber lasers and amplifiers. Praseodymium (Pr3+)‐doped high‐aluminum phosphate (HAP) glasses with excellent chemical durability for thermal ion‐exchanged optical waveguide have been investigated by Tian et al. . In order to improve the solar cell efficiency, potential downconversion was studied in GeS2‐Ga2S3‐CsCl glass for modifying solar spectrum and are found quantum yield to be below 1200 and 1650 nm are 51 and 76%, respectively .
2. Limiting factors in rare earth‐doped glasses
2.1. RE3+ ions solubility in glasses
Higher concentration of RE3+ ions in glasses lead to clusters. Thus, the clusters of rare earth ion serve as luminescent quenchers, either by increasing ion‐ion interactions between rare earth ions or by forming rare earth compounds that are not optically active. Therefore, much effort has been done into developing suitable host glass compositions for various rare earth doping levels. Some of the technological limitations for the development of new glasses are due to the rare earth ion density required for laser action. Currently, high‐power lasers used Nd3+
2.2. Phonon interaction
Since the multiphonon decay process is essentially a competing process to the fluorescence, a low multiphonon decay rate can lead to an increased fluorescence efficiency for many important rare earth transitions. The efficiency of nonradiative transition rate depends on the energy gap between the ground and excited states, as well as the vibrational energy of the oscillators. The nonradiative transition decay rate can be expressed in terms of multiphonon relaxation, concentration quenching, energy transfer to another doping impurity such as transition metal ions or other rare earth ions, and energy transfer to hydroxyl groups OH- . The quenching efficiency is strongly dependent on the number of vibrational quanta that are needed to bridge the gap between the lowest emitting level and the highest nonemitting level of the lanthanide ion. Generally, hosts with low phonon energy tend to have a low multiphonon decay rate; thus, selection of lower phonon hosts such as fluoride or tellurite glasses can reduce the contribution of multiphonon relaxation and allow important radiative transitions.
2.3. Ion‐ion interaction
Ion‐ion interaction is due to multipolar interactions between neighbor rare earth ions. The analysis of ion‐ion interaction and energy transfer provides essential information to the applications of laser glasses and display devices. In such process, the excitation energy transfers from an excited donor to a nearby unexcited activator (acceptor). Many theories have been put forward to give formulas for the rate of energy transfer by electric dipole‐dipole interaction (
Among many energy transfer theories, Förster  and Dexter  theory on energy transfer is one of the most widely employed and the probability rate of energy transfer can be determined as  follows:
where R is the distance of separation between donor and acceptor, CDA is the energy transfer constant (cm6/s), and is the average occupation of phonon mode at temperature T. Then, the energy transfer constant is expressed as follows:
The critical radius of the interaction can be obtained by the product of energy transfer constant and intracenter lifetime of the donor excited level (i.e., ).
In addition to the aforementioned mechanisms, in glasses containing only one RE3+ species (for example Nd3+, Er3+), a number of different ion‐ion interactions occur such as energy migration, cross‐relaxation among others. The most important are outlined below.
2.4. Energy migration
Energy migration is strongly dependent on rare earth ion concentration and due to the dipole‐dipole Förster and Dexter interactions. An excited ion in the metastable state can interact with the nearby ground state ion then promoting it to the excited level (see Figure 3). The successive energy transfers between the ions increase the probability of nonradiative decay that lead to decrease the fluorescence efficiency [40, 41].
2.5. Cross relaxation
Cross relaxation involves the same RE ions and their schematic representation, which is shown in Figure 3. An excited state of ion A that gives half its energy to ion B is in its ground state. So that both ions end up in the intermediate energy level, from which they relax rapidly to the ground state through nonradiative relaxation. This relaxation is usually observed for Nd3+‐doped glasses that cause concentration quenching.
2.6. Upconversion mechanisms
3. Spectroscopic properties of Nd3+‐doped phosphate glasses
3.1. Judd‐Ofelt theory and intensity parameters
Optical spectroscopy often used to measure optical absorption of trivalent rare earth ions in UV‐vis‐NIR regions, from which the effect of a host matrix on the local environment of a given rare earth cation with its first neighbor anions such as oxygen can be elucidated using the theory proposed by Judd  and Ofelt . Each observed transition corresponds to a transition between two spin‐orbit coupling levels. The Judd‐Ofelt theory has been applied for the interpretation of these transitions by the three mechanisms: (1) magnetic dipole transitions, (2) induced electric dipole transitions, and (3) electric quadrupole transitions. The quantitative analysis of the intensities of these f‐f transitions in the rare earth ions has been provided independently by Judd  and Ofelt . The basic idea of Judd and Ofelt is that the intensity of f‐f electric dipole transitions can arise from the admixture into the 4fN configuration of opposite parity (e.g., 4fN-1n1d1 and 4fN-1n1g1). According to Judd‐Ofelt theory, the intensity of magnetic and electric dipole transition is represented as follows:
This means that experimentally measured oscillator strengths could be expressed to a good approximation in terms of absorption of light by electric dipole and magnetic dipole mechanisms. But, the order of magnitude of magnetic dipole oscillator strengths is found to be very low for the observed intensities of rare earth ions and thus will not be considered further. The calculated oscillator strengths are therefore approximately equal to electric dipole oscillator strengths, that is
where υ is the mean energy of the transition , and is the squared reduced matrix element of the unit tensor operator of the rank,
The intensity of an absorption band is expressed in terms of a quantity called the “oscillator strength.” Experimentally, the oscillator strength (f) is a measure of the intensity of an absorption band and is proportional to the area under the absorption peak. The area under an absorption peak is a better measure of the intensity than the molar absorptivity at the peak maximum, because the area is the same for both the resolved and unresolved band. The oscillator strength (f) of each absorption band is expressed in terms of absorption coefficient α(
where m and e are the mass and charge of the electron, c is the velocity of light, and N is the density of the absorbing ions obtained from the rare earth ion concentration and glass density values, respectively. ∫represents the area under the absorption curve. The molar absorptivity of an absorption band at energy ν (cm-1) is given by
where C concentration of rare earth ions per unit volume, optical path length, and is the optical density.
As an example, optical absorption measurements were made at room temperature in the wavelength region 300–900 nm for an Nd3+‐doped phosphate glass using JASCO V‐630, UV‐vis spectrophotometer. Figure 5 shows (a) absorption and (b) emission spectra of Nd3+‐doped phosphate glass. The validity of Judd‐Ofelt theory is determined by the root‐mean‐square (
Using the experimental oscillator strengths (
The covalency between the rare earth ion and the surrounding oxygen in the glass modifies the intensity of hypersensitive transitions (HST), as suggested by Reisfeld and co‐worker [47, 48]. This can be observed more clearly in RE3+‐doped alkali‐ and mixed alkali‐based glasses. For example, in Nd3+ ion, the transition 4I9/2→4G5/2 + 2G7/2 is found to be hypersensitive by selection rule, ΔJ ≤ 2, ΔL ≤ 2, and ΔS = 0. The observed oscillator strengths of the hypersensitive transition are higher when compared to other bands (see inset Figure 5a). Figure 6 shows variation of J‐O parameter, Ω2 with (a) oscillator strength (b) energy (cm-1) of HST transition of Nd3+ ion for alkali, mixed alkali phosphate glasses. From Figure 6a, among the alkali glass matrices, the oscillator strength of HST is found to be lower in lithium phosphate glass matrix and higher in potassium glass matrix. But the oscillator strength of HST is found to be higher in lithium‐potassium phosphate glass matrix among the mixed alkali glass matrices. Thus, the results of oscillator strength show that potassium is playing active role in enhancing the oscillator strengths of Nd3+ ion in potassium phosphate glass matrices (K, Li‐K, and Na‐K) compared to other glass matrices. In lithium phosphate glass matrix, oscillator strength of HST indicates the lower crystal field symmetry at Nd3+ ion site.
The hypersensitive transition can also give the information regarding the covalency nature of rare earth‐ligand interaction, which can be determined by the shift of hypersensitive band position to lower or higher wavelength due to nephelauxetic effect. From Figure 6b, it is observed that for lithium to sodium glass matrices, the peak wavelength of HST shifts toward higher wavelength side and the Ω2 parameter also increases indicating that the structural changes are not influencing the covalence bond. For lithium to potassium and lithium‐potassium glass matrices, the peak wavelength of HST does not change but the Ω 2 parameter increased indicating that the some structural changes are influencing the Nd‐O bond. For sodium to potassium and sodium‐potassium glass matrices, the peak wavelength of HST shifts toward lower wavelength side but Ω2 parameter increased (for Na to K) and decreased (for Na to Na‐K) indicating that the structural changes are influencing the Nd‐O bond.
Due to the zero values of certain reduced matrix elements ‖Uλ‖of Nd3+ ion, certain lasing transitions can be uniquely characterized by the ratio of intensity parameters Ω4 and Ω6, which is known as spectroscopic quality factor (χ) and are shown in Table 2. If χ < 1, the 4F3/2→4I11/2 transition shows stronger intensity than that of 4F3/2→4I9/2 transition. From the Table 2 data, the obtained χ value is <1 for Nd3+‐doped phosphate glasses, indicating that the intensity of 4F3/2→4I11/2 transition at 1064 nm will be stronger for various phosphate glasses .
3.2. Fluorescence analysis and radiative properties
The emission spectra of Nd3+‐doped phosphate glass recorded at room temperature in the wavelength region 800–1500 nm under excitation wavelength, 514.5 nm of Ar3+ laser are shown in Figure 5b. Emission spectra show three emission peaks due to the transitions, 4F3/2→4I9/2, 4F3/2→4I11/2, and 4F3/2→4I13/2 nearly centered at 902, 1069, and 1340 nm, respectively. The stimulated emission cross section is an important parameter and its value is related to the rate of energy extraction from the optical material. The Judd‐Ofelt theory can be applied to laser glasses and can successfully account for the induced emission cross sections that are observed.
The efficiency of a laser transition is evaluated by considering the stimulated emission cross section, and it is related to the radiative transition probability. It can be obtained from the emission spectra using Fuchtbauer‐Ladenburg method 
Where the factor represents the local field correction term for the ion in a medium, υ is the energy of transition, and
The radiative lifetime (τR) of an excited state ψ'J' is calculated from
The fluorescence branching ratio, βR, predicts the relative intensity of lines from a given excited states and characterizes the lasing potency of that particular transition. In order to choose suitable lasing transition, one has to select the transition having branching ratio >0.5 and the energy difference of about 3000 cm-1 between the emitting level and the next lower level. The fluorescence branching ratio (βR) is given by
Table 4 shows critical parameters to the laser designer such as branching ratios and radiative life times, peak stimulated emission cross sections of 1062 nm laser line in various phosphate glasses.
|Glasses||τexp (μs)||τcal (μs)||η (%)||βrad (%)||Δλ (nm)||σp (cm2)|
|0.4MgO‐0.4BaF2‐0.1Al(PO3)3‐0.1Ba(PO3)3 (wt.%) ||185||308||60||49||32||2.97|
4. Rare earth‐doped optical amplifiers
Rare earth‐doped fibers have received growing attention recently. They can be used as amplifiers in optical communication systems and as optical sources. Optical amplifiers amplify an incident weak light signal through the process of stimulated emission. The main ingredient of any optical amplifier is the optical gain realized when the amplifier is optically pumped to achieve population inversion. The optical gain, in general, depends mainly on the doping material, on the frequency (or wavelength) of the incident signal, and also on the local beam intensity at any point inside the amplifier. By a proper choice of the doping materials, the amplifier characteristics such as the operating wavelength and the gain bandwidth can be modified. Many different dopants such as erbium (Er3+), holmium (Ho3+), neodymium (Nd3+), samarium (Sm3+), thulium (Tm3+), and ytterbium (Yb3+) can be used to realize fiber amplifiers operating at different wavelengths covering a wide region extending over 0.5–3.5 μm and the most commonly used hosts are silicate, phosphate, fluoride, and tellurite glasses. Figure 7 shows working of active fibers within a specific wavelength range determined by various rare earth ions. Specially, optical telecommunication transmission [wavelength division multiplexing (WDA)] systems work in the conventional C‐band (1530–1565 nm) telecommunication window. This band can easily be observed in erbium (Er3+) ions among the rare earths and is the most useful dopant for commercial optical amplifiers and erbium‐doped fiber amplifiers (EDFAs) that are made from silicate and phosphate glass matrices. The schematic representation of Er3+‐doped fiber amplifiers (EDFA) is shown in Figure 8. An erbium‐doped fiber is pumped optically by an infrared laser sources at 980 or 1480 nm and are compatible with InGaAs and InGaAsP laser diodes. The three‐level pumping process in EDF is illustrated in Figure 9.
When a laser source tuned at 980 nm is used to pump the EDF, the Er3+ ions move from ground level (4I15/2) to excited level (4I15/2). The ions stay excited level only about 10
Optical pumping provides the necessary population inversion between the energy levels E1 and E2, which in turn provides the optical gain defined as g = σ(N2 - N1), where σ is the transition cross section. Normally, in laser and amplifiers, the gain coefficient decreases as signal power increases and is called as gain saturation. The gain coefficient can be defined as  follows:
where is the small‐signal gain coefficient at a given wavelength, P is the signal power, and Ps is the saturated signal power. The absorption and broadened gain spectra of EDFA (see Figure 10) are the advantages for Wavelength Division Multiplexing (WDM) applications.
Wave division multiplexing optical transmission system requires a flat gain spectrum of EDFA across the whole usable bandwidth. It is difficult to achieve the gain flatness in WDM system because EDFA has the narrow high gain in the C‐hand wavelength region (1530–1570 nm) centered at 1550 nm. In recent decades, many glass hosts for Er3+ ions have been investigated to realize the optical amplifier. For the flattened gain performance of optical amplifier, Er3+
5. Luminescent solar concentrators (LSC)
A schematic of luminescent solar concentrator (LSC) is shown in Figure 11a. LSC is working based on the absorption of sun light by a transparent material that has been doped with high quantum efficiency luminescent ions and subsequently re‐emit by transparent material. The resulting luminescence is propagate by total internal reflection in transparent material and concentrated onto the solar cell, which attached to the edge of the transparent material to convert trapped emission light into electricity. The LSC was first proposed in late 1970s . A typical design consists of a polymer plate doped with a luminescent material, such as a fluorescent organic dye, with solar cells optically matched to the plate edges. In recent decades, luminescent transparent material extends to availability of inorganic luminescence materials such as semiconductor quantum dots (QDs) , rare earth‐doped materials  and semiconductor polymers . Particularly, rare earth‐doped glasses are still great interest due to their potential use as solid‐state lasers and luminescence solar concentrators.
Figure 11b shows emission spectra of (AM1) solar radiation. It is known that the efficiency of solar cell is mainly limited by the loss of photons with much higher energy than the band gap of the photovoltaic solar cell. Normally, photovoltaic cells are made with silicon, which absorb photons only with energy greater than 1.1 eV and it is improving the performance of LSC. The luminescent material usually absorbs all wavelengths below 950 nm. Above 950 nm, the luminescence consists of a strong emission band in the range from 950 to 1000 nm . This region is more reliable to increase the spectral response of the Si Photo‐voltaic cell in LSC (see shaded region in figure). In addition the number of photons in the LSC is double while extending the absorption from visible (300–600 nm) out to the NIR (300–900 nm) range. The extending wavelength increased nonradiative recombination due to increasing molecular dimensions and decreasing probability of radiative transitions . This leads to decrease in fluorescence quantum yield (FQY). In rare earth‐doped materials, the FQY vary greatly depending on host materials and concentration, but values >90% have been reported in glass substrates . The FQY is defined as follows:
A high quantum yield (~95–100%) is essential for good LSC performance. Rare earth ions such as neodymium (Nd3+) and ytterbium (Yb3+) in glassy hosts exhibit high FQY (~90%) values due to range at 800–1300 nm (Nd3+) and 1000 nm (Yb3+) emission peaks. When Nd3+/Yb3+ co‐doped glasses are used as LCS, Nd3+ acts as sensitizer due to its numerous absorption bands in visible region, and Yb3+ acts as activator due to its single emission peak at ~1000 nm. Moreover, this material absorbs 20% of the solar spectrum in the range 440–980 nm range . Figure 12 shows absorption (for Nd3+) and emission (for Nd3+, Yb3+) spectra for realizing the LCS. It is observed that the emission peak at ~1000 nm is matched perfectly to the maximum spectral response of a Si‐Solar cell.
In summary, this chapter consists of a brief discussion on electronic energy‐level structure of RE3+ in solids, structural features, and general considerations in lasers glasses such concentration quenching, phonon interaction, ion‐ion interaction, and upconversion mechanisms. Judd‐Ofelt intensity parameters (Ωλ, λ = 2, 4, and 6) on Nd3+‐doped phosphate glasses and relevant theory were considered. We also included a study on the covalency between rare earth ion and the surrounding oxygen in the glass that increases the intensity of hypersensitive transitions for the case of alkali‐ and mixed alkali phosphate‐based glasses. Laser parameters such as emission cross sections (σp), radiative lifetime (τ), branching ratios (β), peak bandwidth (Δλ), and quantum efficiency on Nd3+‐doped phosphate glasses are reported. Laser emission process in three‐level and two‐level‐based silica‐EDFA was discussed as well as significant features of rare earth‐doped luminescent solar concentrators.
The authors would like to thank to Conselho Nacional de Desenvolvimento Científico e Tecnológico (CNPq) and Coordenação de Aperfeiçoamento de Pessoal de Nível Superior (CAPES), PNPD/CAPES, and FAPEMIG.
Moulton P.F. Laser Hand Book, 5th ed. M. Bass and M. L. Stitch. Netherland Publishers: Amsterdam; 1985. 203 p.
Sutton D. Electron Spectra of Transition Metal Complexes. McGraw‐Hill Publishing Company Ltd: New York; 1969.
Belançon M.P., Marconi J.D., Ando M.F., Barbosa L.C. Near‐IR emission in Pr3+ single doped and tunable near‐IR emission in Pr3+/Yb3+ codoped tellurite tungstate glasses for broadband optical amplifiers. Opt. Mater. 2014; 36: 1020–1026. doi:10.1016/j.optmat.2014.01.014
Balakrishna A., Rajesh D., Ratnakaram Y.C. Structural and optical properties of Nd3+ in lithium fluoro‐borate glass with relevant modifier oxides. Opt. Mater. 2013; 35: 2670–2676. doi:10.1016/j.optmat.2013.08.004
Vishwakarma A.K., Jayasimhadri M. Significant enhancement in photoluminescent properties via flux assisted Eu3+ doped BaNb2O6 phosphor for white LEDs. J. Alloys Compound. 2016; 683: 379–386. doi:10.1016/j.jallcom.2016.05.052
Gao Y., Hu Y., Ren P., Zhou D., Qiu J. Phase transformation and enhancement of luminescence in the Tb3+‐Yb3+ co‐doped oxyfluoride glass ceramics containing NaYF4 nanocrystals. J. Eur. Ceramic Soc. 2016; 36: 2825–2830. doi:10.1016/j.jeurceramsoc.2016.04.027
Guo H., Liu L., Wang Y., Hou C., Li W., Lu M., Zou K., Peng B. Host dependence of spectroscopic properties of Dy3+ ‐ doped and Dy3+, Tm3+‐codoped Ge–Ga–SCdI2 chalcohalide glasses. Opt. Express. 2009; 17: 15350–15358. doi:10.1364/OE.17.015350
Seshadri M., Chillcce E.F., Marconi J.D., Sigoli F.A., Ratnakaram Y.C., Barbosa L.C. Optical characterization, infrared emission and visible up‐conversion in Er3+ doped tellurite glasses. J. Non‐Cryst. Solids. 2014; 402: 141–148. doi:10.1016/j.jnoncrysol.2014.05.024
Diek G.H. Spectra and Energy Levels of Rera Earth Ions in Crystals. New York, Wiley: 1968.
Peacock R.D. Rare earths. In: Structure and Bond, vol. 22. Springer, Berlin: 1975; p. 83.
Reisfeld R. Radiative and nonradiative transition of rare earths in glasses. In: Structure and Bond, vol. 22. Springer, Berlin: 1975; p. 123.
Wybourne B.G. Spectroscopy Properties of Rare earths. New York, Wiley: 1965.
ASTM Standards on Glass and Glass Products, prepared by ASTM Committee C14, American Society for Testing Materials, April 1955.
Shelby J.E. Introduction to Glass Science and Technology, 2nd ed. Royal Society of Chemistry; Cambridge: 2005; 291 p.
Zachariasen W.H. The atomic arrangement in glasses. J. Am. Chem. Soc. 1932; 54: 3841–3851.
Herrmann A., Kuhn S., Tiegel M., Russel C., Korner J., Klopfel D., Hein J., Kaluza M.C. Structure and fluorescence properties of ternary aluminosilicate glasses doped with samarium and europium. J. Mater. Chem. C. 2014; 2: 4328–4337. doi:10.1039/C4TC00036F
Tiegel M., Herrmann A., Russel C., Korner J., Klopfel D., Hein J., Kaluza M.C. Magnesium aluminosilicate glasses as potential laser host material for ultrahigh power laser systems. J. Mater. Chem. C. 2013; 1: 5031–5039. doi:10.1039/C3TC30761A
Seshadri M., Barbosa L.C., Radha M. Study on structural, optical and gain properties of 1.2 and 2.0 μm emission transitions in Ho3+ doped tellurite glasses. J. Non‐Cryst. Solids. 2014; 406: 62–72. doi:10.1016/j.jnoncrysol.2014.09.042
Van Wazer J.R. Phosphorous and Its Compounds, vol. 1. New York, Interscience; 1958.
Kordes E., Vogel W., Feterowsky R. Physical chemistry studies About the properties and Feinban of phosphate glasses. Z. Elektrochem. 1953; 57: 282.
Kordes E., Nieder R. Glasstech. 1968; 41: 41.
Kordes E., Vogel W., Feterowsky R. Z. Elektrochem. 1953; 57: 282.
Hench L.L. Bioceramics. J. Am. Ceram. Soc. 1991; 74: 1487.
Volksch G., Hoche T., Szabo I., Holand W., Glasstech. Ber. Glass Sci. Technol. 1998; 71: 500.
Pinheiro A.S., Freitas A.M., Silva G.H., Bell M.J.V, Anjos V., Carmo A.P., Dantas N.O. Laser performance parameters of Yb3+ doped UV‐transparent phosphate glasses. Chem. Phys. Lett. 2014; 592: 164–169. doi:10.1016/j.cplett.2013.12.022
Silva G.H., Anjos V., Bell M.J.V., Carmo A.P., Pinheiro A.S. Dantas N.O. Eu3+ emission in phosphate glasses with high UV transparency. J. Lumin. 2014; 154: 294–297. doi:10.1016/j.jlumin.2014.04.043
Deutschbein O., Pautrat C., Svirchevsky I.M. Phosphate glasses: New laser materials. Rev. Phys. Appl. 1967; 1: 29.
Abd El‐Ati M.I., Higazy A.A. Electrical conductivity and optical properties of gamma‐irradiated niobiumphosphate glasses. J. Mater. Sci. 2000; 35: 6175. doi:10.1023/A:1026768925365
Pinheiro A.S., da Costa Z.M., Bell M.J.V., Anjos V., Dantas N.O., Reis S.T. Thermal characterization of iron phosphate glasses for nuclear waste disposal. Opt. Mater. 2011; 33: 1975–1979. doi:10.1016/j.optmat.2011.03.050
Martin S.W. J. Review of the Structures of Phosphate Glasses. Solid State Chem. 1991; 28: 163.
Belliveau T.F., Simkin D.J. On the coordination environment of rare earth ions in oxide glasses: Calcium titanosilicate and sodium aluminosilicate glasses. J. Non‐Cryst. Solids. 1989; 110:127. doi:10.1016/0022‐3093(89)90249‐4
Babu S., Seshadri M., Reddy Prasad V., Ratnakaram Y.C. Spectroscopic and laser properties of Er3+ doped fluoro‐phosphate glasses as promising candidates for broadband optical fiber lasers and amplifiers. Mater. Res. Bulletin. 2015; 70: 935–944. doi:10.1016/j.materresbull.2015.06.033
Tian Y.M., Shen L.F., Pun E.Y.B., Lin H. High‐aluminum phosphate glasses for single‐mode waveguide‐typed red light source. J. Non‐Cryst. Solids. 2015; 426: 25–31. doi:10.1016/j.jnoncrysol.2015.06.015
Fan B., Point C., Adam J.L., Zhang X., Fan X., Ma H. Near‐infrared down‐conversion in rare earth‐doped chloro‐sulfide glass GeS2‐Ga2S3‐CsCl: Er, Yb. J. Appl. Phys. 2011; 110: 13107. doi:10.1063/1.3665638
Ehrmann P.R., Campbell J.H. Nonradiative energy losses and radiation trapping in neodymium‐doped phosphate laser glasses. J. Am. Ceram. Soc. 2002; 85: 1061–1069. doi:10.1111/j.1151‐2916.2002.tb00223.x
Goncalves R.R., Carturan G., Montagna M., Ferrari M., Zampedri L., Pelli S., Righini G.C., Ribeiro S.J.L., Messaddeq Y. Erbium-activated HfO2-based waveguides for photonics Opt. Mater. 2004; 25: 131–139. doi:10.1016/S0925‐3467(03)00261‐1
Förster T. Zwischenmolekulare Energiewanderung und Fluoreszenz. Ann. Phys. 1948; 2: 55–75.
Dexter D.L. A theory of sensitized luminescence in solids. J. Chem. Phys. 1953; 21: 836–850. doi:10.1063/1.1699044
Tarelho T.V.G. Gomes L., Ranieri I.M. Determination of microscopic parameters for nonresonant energy‐transfer processes in rare earth‐doped crystals. Phys. Rev. B. 1997; 56: 14344. doi:10.1103/PhysRevB.56.14344
de Sousa D. F., Batalioto F., Bell M.J.V., Oliveira S.L., Nunes L.A.O. Spectroscopy of Nd3+ and Yb3+ codoped fluoroindogallate glasses. J. Appl. Phys. 2001; 90: 3308–3313. 10.1063/1.1397289
Batalioto F., de Sousa D.F., Bell M.J.V., Lebullenger R., Hernandes A.C., Nunes L.A.O. Optical measurements of Nd3+/Yb3+ codoped fluoroindogallate glasses. J. Non‐Cryst. Solids. 2000; 273: 233–238. doi:10.1016/S0022‐3093(00)00132‐0
Judd B.R. Optical absorptionm intensities of rare earth ions. Phys. Rev. 1962; 127: 750. doi:10.1103/PhysRev.127.750
Ofelt G.S. Intensities of crystal spectra o rare earth ions. J. Chem. Phys. 1962; 37: 511. doi:10.1063/1.1701366
Broer L.F.J., Gorter C.J., Hoogschangen J. The intensities and multiple character in the spectra of rare earth ions. Physica 1945; XI:231–250.
Seshadri M., Venkata Rao K., Lakshmana Rao J., Koteswara Rao K.S.R., Ratnakaram Y.C. Spectroscopic investigations and luminescence spectra of Nd3+ and Dy3+ doped different phosphate glasses. J. Lumin. 2010; 130: 536–543. doi:10.1016/j.jlumin.2009.10.027
Ratnakaram Y.C., Thirupathi Naidu D., Vijaya Kumar A., Rao J.L. Characterization of Tm3+ doped mixed alkali borate glasses ‐ Spectroscopic investigations. J. Phys. Chem. Solids. 2003; 64 (12): 2487–2495. doi:10.1016/j.jpcs.2003.06.001
Reisfeld R., Jorgensen C.K. Lasers and excited states of rare earths. Berlin, Springer‐Verlag; 1977.
Oomen E.W.J.L., Van Dongen A.M.A. Europium (III) in oxide glasses: dependence of the emission spectrum upon glass composition. J. Non‐Cryst. Solids. 1989; 111: 205–213. doi:10.1016/0022‐3093(89)90282‐2
Martins V.M., Messias D.N., Doualan J.L., Braud A., Camy P., Dantas N.O., Catunda T., Pilla V., Andrade A.A., Moncorgé R. Thermo‐optical properties of Nd3+ doped phosphate glass determined by thermal lens and lifetime measurements. J. Lumin. 2016; 162: 104–107. doi:10.1016/j.jlumin.2015.02.013
Linganna K., Dwaraka Viswanath C.S., Narro‐Garcia R., Ju S., Han W.T., Jayasankar C.K., Venkatramu V. Thermal and optical properties of Nd3+ ions in K‐Ca‐Al fluorophosphate glasses. J. Lumin. 2015; 166: 328–334. doi:10.1016/j.jlumin.2015.05.024
Upendra Kumar K., Babu P., Jang K.H., Jin Seo H., Jayasankar C.K., Joshi A.S. Spectroscopic and 1.06m laser properties of Nd3+‐doped K‐Sr‐Al phosphate and fluorophosphate glasses. J. Alloys and Compd. 2008; 458: 509–516. doi:10.1016/j.jallcom.2007.04.035
Binnemans K., Van Deun R., Gorller‐Walrand C., Adam J.L. Optical properties of Nd3+ ‐doped fluorophosphate glasses. J. Alloys and Compounds. 1998; 275–277: 455–460. doi:10.1016/S0925‐8388(98)00367‐3
Tian C., Chen X., Shuibao Y. Concentration dependence of spectroscopic properties and energy transfer analysis in Nd3+ doped bismuth silicate glasses. Solid State Sci. 2015; 48: 171–176. doi:10.1016/j.solidstatesciences.2015.08.008
Seshadri M., Barbosa L.C., Cordeiro C.M.B., Radha M., Sigoli F.A., Ratnakaram Y.C. Study of optical absorption, visible emission and NIR‐Vis luminescence spectra of Tm3+/Yb3+, Ho3+/Yb3+ and Tm3+/Ho3+/Yb3+ doped tellurite glasses. J. Lumin. 2015; 166: 8–16. doi:10.1016/j.jlumin.2015.04.022
Balakrishnaiah R., Babu P., Jayasankar C.K., Joshi A.S., Speghini A., Bettinelli M. Optical and luminescence properties of Nd3+ ions in K‐Ba‐Al phosphate and fluorophosphate glasses. J. Phys.: Condens. Matter. 2006; 18: 165–179. doi:10.1088/0953‐8984/ 18/1/012
Surendra babu S., Babu P., Jayasankar C.K., Joshi A.S., Speghini A., Bettinelli M. Luminescence and optical absorption properties of Nd3+ ions in K‐Mg‐Al phosphate and fluorophosphate glasses. J. Phys.: Condens. Matter. 2006; 18: 3975–3991. doi:10.1088/0953‐8984/ 18/16/007
Ajroud M., Haouari M., Ben Ouada H., Maaref H., Brenier A., Garapon C. Investigation of the spectroscopic properties of Nd3+‐doped phosphate glasses. J. Phys.: Condens. Matter. 2000; 12: 3181–3193. doi:10.1088/0953‐8984/12/13/324
Choi J.H., Margaryan A., Margaryan A., Shi F.G. Judd‐Ofelt analysis of spectroscopic properties of Nd3+‐doped novel fluorophosphate glass. J. Lumin. 2005; 114: 167–177. doi:10.1016/j.jlumin.2004.12.015
Advanced Optics, SCHOTT North America Inc., Duryea, PA, USA.
HOYA Corporation USA, Optics Division, 3285 Scott Blvd., Santa Clara, CA 95054 USA.
KIGRE, Inc., 100 Marshland Road, Hilton Head, SC 29926, USA.
lizuka K. Lab instruction notes for “Erbium Doped Fiber Amplifiers”. University of Toronto; Canada: 1998.
Wang J.S., Vogel E.M., Snitzer E. Terullite glass: a new candidate for fiber devices. Opt. Mater. 1994; 3(3): 187–203. doi:10.1016/0925‐3467(94)90004‐3
Mori A., Ohishi Y., Sudoi S. Erbium‐doped tellurite‐based fiber laser and amplifier. Electron. Lett. 1997; 33(10); 863–865.
Sugimoto N., Ochiai K., Ohara S., Hayashi H., Fukasawa Y., Hirose T., Reyes M. Highly efficient and short length Lanthanum codoped Bh03‐based EDF for extended L‐band amplification. In: Proceedings of Optical Amplifiers and their applications. 2002, OAA’02, PD 5, Vancouver, 2002.
Weber W.H., Lambe J. Luminescent greenhouse collector for solar radiation. Appl. Opt. 1976; 15(10): 2299–2300. doi:10.1364/AO.15.002299
Barnham K., Marques J.L., Hassard J., Obrien P. Quantum‐dot concentrator and thermodynamic model for the global redshift. Appl. Phys. Lett. 2000; 76(9): 1197–1199. doi:10.1063/1.125981
Werts M.H.V., Hofstraat J.W., Geurts F.A.J., Verhoeven J.W. Fluorescein and eosin as sensitizing chromophores in near‐infrared luminescent ytterbium(III), neodymium(III) and erbium(III) chelates. Chem. Phys. Lett. 1997; 276(3/4): 196–201. doi:10.1016/S0009‐2614(97)00800‐2
Sholin V., Olson J.D., Carter S.A. Semiconducting polymers and quantum dots in luminescent solar concentrators for solar energy harvesting. J. Appl. Phys. 2007; 101: 1231141–1231149. doi:10.1063/1.2748350
Brenda C.R., Wilson L.R., Richards B.S. Advanced material concepts for luminescent solar concentrators. IEEE J. Selected Topics in Quant. Electron. 14(5): 2008; 1321–1322.
Goetzberger A., Greubel W. Solar energy conversion with fluorescent collectors. Appl. Phys. 1977; 14: 123–139. doi:10.1007/BF00883080
Reisfeld R. Future technological applications of rare earth doped materials. J. Less Common Mater. 1983; 93: 243–251. doi:10.1016/0022‐5088(83)90163‐7